Journal Pre-proofs Predicting New Iron Garnet Thin Films with Perpendicular Magnetic Anisotropy Saeedeh Mokarian Zanjani, Mehmet C. Onbaşlı PII: DOI: Reference:
S0304-8853(19)31915-8 https://doi.org/10.1016/j.jmmm.2019.166108 MAGMA 166108
To appear in:
Journal of Magnetism and Magnetic Materials
Received Date: Revised Date: Accepted Date:
31 May 2019 1 October 2019 4 November 2019
Please cite this article as: S. Mokarian Zanjani, M.C. Onbaşlı, Predicting New Iron Garnet Thin Films with Perpendicular Magnetic Anisotropy, Journal of Magnetism and Magnetic Materials (2019), doi: https://doi.org/ 10.1016/j.jmmm.2019.166108
This is a PDF file of an article that has undergone enhancements after acceptance, such as the addition of a cover page and metadata, and formatting for readability, but it is not yet the definitive version of record. This version will undergo additional copyediting, typesetting and review before it is published in its final form, but we are providing this version to give early visibility of the article. Please note that, during the production process, errors may be discovered which could affect the content, and all legal disclaimers that apply to the journal pertain.
© 2019 Published by Elsevier B.V.
Predicting New Iron Garnet Thin Films with Perpendicular Magnetic Anisotropy Saeedeh Mokarian Zanjani1, Mehmet C. Onbaşlı1,2,*
Graduate School of Materials Science and Engineering, Koç University, Sarıyer, 34450 Istanbul, Turkey. 2 Department of Electrical and Electronics Engineering, Koç University, Sarıyer, 34450 Istanbul, Turkey. * Corresponding Author: [email protected]
Abstract: Magnetic iron garnets are insulators with low Gilbert damping with many applications in spintronics. Many emerging spintronic applications require perpendicular magnetic anisotropy (PMA) although garnets have only a few PMA types (i.e. terbium and samarium garnet). More and stable PMA garnet options are needed for investigating new spintronic phenomena. In this study, we predict 20 new epitaxial magnetic iron garnet film/substrate pairs with stable PMA at room temperature. The effective anisotropy energies of 10 different garnet films that are latticematched to 5 different commercially available garnet substrates (total 50 film/substrate pairs) have been calculated using shape, magnetoelastic and magnetocrystalline anisotropy terms. Strain type, tensile or compressive depending on substrate choice, as well as the sign and the magnitude of the magnetostriction constants of garnets determine if a garnet film may possess PMA. We show the conditions in which Samarium, Gadolinium, Terbium, Holmium, Dysprosium and Thulium garnets may possess PMA on the investigated garnet substrate types. New PMA garnet films with tunable saturation moment and field may improve spin-orbit torque memory and compensated magnonic thin film devices. Keywords: rare earth iron garnets, thin film, perpendicular magnetic anisotropy.
1. Introduction With the development of sputtering and pulsed laser deposition (PLD) of high-quality iron garnet thin films with ultralow Gilbert damping, researchers have been able to investigate a wide variety of magnetization switching and spin wave phenomena [1-3]. The key enabler in many of these studies has been Yttrium iron garnet (Y3Fe5O12, YIG)  which has a very low Gilbert damping allowing spin waves to propagate over multiple millimeters across chip. YIG thin films are useful for spin wave device applications, but since their easy axes lie along film plane, their utility cannot be extended to different mechanisms such as spin-orbit torques, Rashba-Edelstein effect, logic devices, forward volume magnetostatic spin waves . At the same time, to have reliable and fast response using low current densities as in spin-orbit torque switching, magnetization orientation needs to be perpendicular to the surface plane . There is a number of studies on tuning anisotropy or obtaining perpendicular magnetic anisotropy (PMA) in insulator thin films [6-11]. Among the materials studied, insulating magnetic garnets whose magnetic properties can be tuned have been a matter of interest over the past decades  due to their low damping and high magnetooptical Faraday rotation. In order to obtain PMA in magnetic garnets, one needs to engineer the anisotropy terms that give rise to out-of-plane easy axis. Controlling magnetic anisotropy in thin film garnets offers researchers different testbeds for experimenting new PMA-based switching phenomena. In addition, it allows investigation of anisotropy-driven ultrafast dynamic magnetic response in thin films and nanostructures. YIG films as the most common REIG display in-plane easy axis because of their large shape anisotropy and negligible magnetocrystalline anisotropy. Although PMA of ultrathin epitaxial YIG films has been reported [15, 16], the tolerance for fabrication condition variations for PMA YIG is very limited and strain effects were found to change magnetocrystalline anisotropy in YIG. In case of YIG thin film grown on Gadolinium Gallium Garnet (GGG), only partial anisotropy control has been possible through significant change in oxygen stoichiometry , which increases damping. Since the fabrication of high-quality and highly PMA YIG films is not easy for practical thicknesses on gadolinium gallium garnet substrates (GGG), researchers have explored tuning magnetic anisotropy by substituting Yttrium sites with other rare earth elements [18, 19]. New garnet thin films that can exhibit PMA with different coercivities, saturation fields, compensation points and tunable Gilbert damping values must be developed in order to evaluate the effect of these parameters on optimized spintronic insulator devices. Since the dominant anisotropy energy term is shape anisotropy in thin film YIG, some studies focus on reducing the shape anisotropy contribution by micro and nanopatterning [20-22]. Continuous YIG films were etched to form rectangular nanostrips with nanometer-scale thicknesses, as schematically shown on Fig. 1(a). Thus, least magnetic saturation field is needed along the longest dimension of YIG nanostrips. As the length-to-thickness ratio decreases, the effect of shape anisotropy is reduced through the film thickness and in-plane easy axis is converted to PMA .
While reducing the effect of shape anisotropy is necessary, one also needs to use magnetoelastic (ME) anisotropy contribution to reorient magnetic easy axis towards out of film plane, as schematically shown on Fig. 1(b). Strain-induced magnetic anisotropy has been studied previously in bulk garnets and metallic systems [23, 24]. Strain-induced PMA in rare earth (RE) iron garnets, especially in YIG, has been demonstrated to overcome shape anisotropy [15, 16, 25, 26]. If ME anisotropy term induced by crystal lattice mismatch is larger than shape anisotropy and has opposite sign, then it overcomes shape. Thus, the easy axis of the film becomes perpendicular to the film plane and the hysteresis loop becomes square-shaped with low saturation field . One can also achieve PMA in other RE magnetic iron garnets due to their lattice parameter mismatch with their substrates. PMA has previously been achieved using Substituted Gadolinium Gallium Garnet (SGGG) as substrate and a Samarium Gallium Garnet (SmGG) ultrathin film as buffer layer under (and on) YIG . In Ref.[7, 17], the authors reported that if magnetostriction coefficient (λ111) is negative and large enough to overcome shape anisotropy, and tensile strain is introduced to the thin film sample (ε||>0), the easy axis becomes perpendicular to the sample plane as in the case of Thulium iron garnet (Tm3Fe5O12, TmIG). A different form of ME anisotropy effect can be induced by using porosity in garnet thin films. Mesoporous Holmium Iron Garnet (Ho3Fe5O12, HoIG) thin film on Si (001) exhibits PMA due to reduced shape anisotropy, increased magnetostrictive and growth-induced anisotropy effects. Such combined effects lead to PMA in HoIG. The pore-solid architecture itself imposes an intrinsic strain on the solution processed garnet film. This example indicates that the film structure can be engineered in addition to the substrate choices in order to overcome shape anisotropy in thin film iron garnets. Another key method for controlling anisotropy is strain doping through substitutional elements and using their growth-induced anisotropy effects, as schematically shown on Fig. 1(c). Bi-doped yttrium iron garnet (Bi:YIG and Bi:GdIG) was shown to have PMA at increased annealing temperature due to the chemical composition change [19, 28]. Another reason for PMA in these thin films is strain from GGG substrate . Doping of oxides by Helium implantation was shown to reversibly and locally tune magnetic anisotropy . For TbxY3-xFe5O12 (x=2.5, 2.0, 1.0, 0.37) samples grown by spontaneous nucleation technique , magnetic easy axis was found to change from  to  direction as Tb concentration was decreased. The first-order anisotropy constant K1 undergoes a change of sign near 190K. Another temperature-dependent lattice distortion effect that caused anisotropy change was also reported for YIG films . These results indicate that temperature also plays an important role in both magnetic compensation, lattice distortion and change in anisotropy. In this study, we systematically calculate the anisotropy energies of 10 different types of latticematched iron garnet compounds epitaxially-grown as thin films (X3Fe5O12, X = Y, Tm, Dy, Ho, Er, Yb, Tb, Gd, Sm, Eu) on commercially available (111)-oriented garnet substrates (Gd3Ga5O12GGG, Y3Al5O12-YAG, Gd3Sc2Ga3O12 -SGGG, Tb3Ga5O12 –TGG, Nd3Ga5O12 -NGG). Out of the 3
50 different film/substrate pairs, we found that 20 cases are candidates for room temperature PMA. Out of these 20 cases, 7 film/substrate pairs were experimentally tested and shown to exhibit characteristics originating from PMA. The remaining 13 pairs, to the best of our knowledge, have not been tested for PMA experimentally. We indicate through systematic anisotropy calculations that large strain-induced magnetic anisotropy terms may overcome shape when the films are highly strained. We use only the room temperature values of λ111 and only report predictions for room temperature (300K). Throughout the rest of this study, the films are labelled as XIG (X = Y, Tm, Dy, Ho, Er, Yb, Tb, Gd, Sm, Eu), i.e. TbIG (Terbium iron garnet) or SmIG (Samarium iron garnet) etc. to distinguish them based on the rare earth element. Our model could accurately predict the magnetic easy axis in almost all experimentally tested garnet film/substrate cases provided that the actual film properties are entered in the model and that the experimental film properties satisfy cubic lattice matching condition to the substrate.
Fig. 1. Methods to achieve perpendicular magnetic anisotropy in iron garnet thin films. (a) Micro/nano-patterning reduces shape anisotropy and magnetoelastic anisotropies overcome shape. (b) Large strain-induced anisotropy must overcome shape anisotropy to yield out-of-plane easy axis. (c) Substitutional doping in garnets overcome shape anisotropy by enhancing magnetocrystalline, growthinduced or magnetoelastic terms.
2. Methods 2.1. Anisotropy energy density calculations Total anisotropy energy density contains three main contributions; according the Eq.1, shape anisotropy (Kshape), first order cubic magnetocrystalline anisotropy (K1), and strain-induced 5
(magnetoelastic) anisotropy (Kindu) parameters determine the total effective anisotropy energy density . (1)
Keff = Kindu + Kshape + K1
In case of garnet film grown on a (111) substrate, the ME anisotropy energy density, resulting from magneto-elastic coupling is calculated by Eq.2: 3
Kindu = ― 2λ111σ||
where λ111 is magnetostriction constant along  direction and it is usually negative at room temperature . In Eq.2, σ|| is the in-plane stress induced in the material as a result of lattice mismatch between film and the substrate, and it is calculated from Eq.3 : Y
σ|| = 1 ― νε|| where Y is elastic modulus, and ν is Poisson’s ratio .
For calculation of in-plane strain, lattice parameter values obtained from the XRD characterization of the thin films are used. Eq.4 shows the strain relation as the lattice constant difference between the bulk form of the film and that of the substrate divided by the lattice constant for the bulk form of the film. ε|| =
afilm ― abulk
Assuming the lattice parameter of the thin film matches with that of the substrate, the lattice constant of substrate can be used as the lattice constant of thin film for calculation of strain in Eq. 5 : ε|| =
asub ― afilm
The lattice constants used for the films and substrates examined for this study are presented on Table 1. Shape anisotropy depends on the geometry and the intrinsic saturation magnetic moment of the iron garnet material. Shape anisotropy has a demagnetizing effect on the total anisotropy. This significant anisotropy effect can be observed in magnetic hysteresis loops and FMR measurements . For continuous films, the shape anisotropy is calculated as : Kshape = 2πM2s
By obtaining the values of Ms for rare earth iron garnets as a function of temperature [38, 39], the value for shape anisotropy energy density have been calculated using Eq.6.
Intrinsic magnetic anisotropy , so called magnetocrystalline anisotropy, has the weakest contribution to anisotropy energy density compared to shape, and strain-induced anisotropies [8, 10, 15, 17]. The values for the first order magnetocrystalline anisotropy is calculated and reported previously for rare earth iron garnets at different temperatures . A key consideration in magnetic thin films is saturation field. In anisotropic magnetic thin films, the anisotropy fields have also been calculated using Eq.7 as a measure of how much field the films need for magnetic saturation along the easy axis: Keff
HA = 2 Ms
Table 1. List of magnetic rare earth iron garnet thin films and garnet substrates available off-the-shelf used for this study. The fourth column shows the lattice constants used for calculating the magnetoelastic anisotropy values of epitaxial garnets on the given substrates.
Garnet Chemical material formula GGG Gd3Ga5O12 YAG Y3Al5O12 SGGG Gd3Sc2Ga3O12 TGG Tb3Ga5O12 NGG Nd3Ga5O12 YIG Y3Fe5O12 TmIG Tm3Fe5O12 DyIG Dy3Fe5O12 HoIG Ho3Fe5O12 ErIG Er3Fe5O12 YbIG Yb3Fe5O12 TbIG Tb3Fe5O12 GdIG Gd3Fe5O12 SmIG Sm3Fe5O12 EuIG Eu3Fe5O12 3. Results and Discussion
Purpose Substrate Substrate Substrate Substrate Substrate Film Film Film Film Film Film Film Film Film Film
Bulk lattice constant (Å) 12.383 12.005 12.480 12.355 12.520 12.376 12.324 12.440 12.400 12.350 12.300 12.460 12.480 12.530 12.500
Tables 1 and 2 list in detail the parameters used and the calculated anisotropy energy density terms for magnetic rare earth iron garnets at 300K. These tables show only the cases predicted to be PMA out of a total of 50 film/substrate pairs investigated. The extended version of Tables 1 and 2 for calculated anisotropy energy density terms of all 50 film/substrate pairs are provided in the Data in Brief tables. The tabulated values for saturation magnetization, Ms, [38, 39] and lattice parameters  have been used for the calculations. In this study, we assumed the value of Young’s modulus and Poisson ratio as 2.00×1012 dyne·cm-2 and 0.29 for all garnet types, 7
respectively, based on Ref.. We also assume that the Ms, used for calculation of shape anisotropy, does not change with the film thickness. Table 2. Anisotropy energy density parameters calculation results. REIG on GGG (as=12.383Å), YAG (Y3Al5O12, as=12.005Å), SGGG (as=12.48Å) and TGG (Tb3Ga5O12, as=12.355Å), and NGG (Nd3Ga5O12, as=12.509Å) substrates, with Keff < 0, are presented. Ms (film saturation moment) and Kshape (shape anisotropy for the films) are on the third and fourth columns, respectively. The stress σ calculated using Eq. 3 for fully lattice-matched films and the magnetostriction constants of the films, λ111, are on columns 6 and 7. Magnetoelastic anisotropy Kindu, magnetocrystalline anisotropy K1, and the total magnetic anisotropy energy Keff are calculated and listed on columns 8, 9 and 10. HA (column 11) is the anisotropy field (the field required to saturate the films). Film
K1 (300K) (erg·cm-3) (× 103) -5.00
Kshape (erg·cm-3) (× 103)
ε|| (× 103)
σ|| (dyn·cm-2) (×1010)
Kindu (erg·cm-3) (×104)
Keff (erg·cm-3) (× 103)
HA (Oe) (× 103)
In this study, we take the same sign convention as in Ref. . The films exhibit PMA when Keff < 0. So for obtaining PMA, negative and large values for anisotropy energy density are desired. As all the garnets (except TbIG) possess negative λ111 at room temperature, the sign of the strain (tensile or compressive) determines whether the induced anisotropy is negative or positive. In the literature [15, 18, 43, 44] however, we observe that PMA was defined for either positive or 8
negative effective anisotropy energy density (Keff). This inconsistency may cause confusion among researchers. Thermodynamically, a higher energy means an unstable state with respect to lower energy cases. Easy axis, by definition, is the axis along which the magnetic material can be saturated with lowest external field or lowest total energy. A magnetic material would thus spontaneously minimize its energy and reorient its magnetic moment along the easy axis. As a result, we use here Keff < 0 for out-of-plane easy axis. Due to the thermodynamic arguments mentioned above, we suggest researchers to use Keff < 0 definition for PMA. 3.1. Effect of Substrate on Anisotropy Energy Density Changing the substrate alters the strain in the film, which also Kindu. Fig.2 shows the calculated anisotropy energy density of REIG thin films grown on five commercially available different substrates: Gadolinium Gallium Garnet (Gd3Ga5O12, GGG), Yttrium Aluminum Garnet (Y3Al5O12, YAG), Substituted Gadolinium Gallium Garnet (Gd3Sc2Ga3O12, SGGG), Terbium Gallium Garnet (Tb3Ga5O12, TGG), and Neodymium Gallium Garnet (Nd3Ga5O12, NGG). As shown on Fig. 2(a), when grown on GGG substrate, DyIG, HoIG, GdIG, and SmIG possess compressive strain (afilm>asubstrate). Considering the large negative λ111 for each case, the Kindu values are estimated to cause negative total effective anisotropy energy density. As a result, DyIG, HoIG, GdIG, and SmIG on GGG are predicted to be PMA cases. Based on our calculations, TmIG on GGG (111) is estimated to be in-plane easy axis although unambiguous experimental evidence indicates that TmIG grows with PMA on GGG (111) [17, 18]. The fact that only considering shape, magnetocrystalline and magnetoelastic anisotropy terms does not verify the anisotropy state of TmIG. This experimental result suggests that the PMA in TmIG/GGG (111) may originate from a different anisotropy term such as surface anisotropy, growth-induced or stoichiometry-driven anisotropy. Since the films used in the experiments are less than 10 nm or 5-8 unit cells thick, surface effects may become more significant.
Fig. 2. Calculated effective anisotropy values for each rare earth iron garnet thin film when they are epitaxially grown on (a) GGG, (b) YAG, (c) SGGG, (d) TGG, (e) NGG substrates. Note that the scales of the axes are different in each part.
Yttrium Aluminum Garnet (YAG) is a substrate with smaller lattice parameter than all the REIG films considered. With a substrate lattice parameter of as=12.005Å, YAG causes significant and 10
varying amounts of strain on YIG (af=12.376Å), TmIG (af=12.324Å), DyIG (af=12.440Å), HoIG (af=12.400Å), ErIG (af=12.350Å), YbIG (af=12.300Å), TbIG (af=12.460Å), GdIG (af=12.480Å), SmIG (af=12.530Å) and EuIG (af=12.500Å). Strain from YAG substrate yields negative Kindu for these films, and it overcomes the shape anisotropy in these garnets when they are grown on YAG. Consequently, Keff values become negative and these garnet films are estimated to possess PMA. In the exceptional cases of TbIG, EuIG, compressive strain is not enough to induce negative strain anisotropy because the magnetostriction coefficients of TbIG and EuIG are positive. So the Kindu terms are also positive for both TbIG (Kindu(TbIG) = 1.85×106 erg·cm-3) and EuIG (Kindu(EuIG) = 3.01×105 erg·cm-3) and do not yield PMA. Other potential PMA garnet films on SGGG substrate are GdIG, TbIG, and SmIG. TbIG and GdIG cases are particularly interesting as growth conditions of these materials can be further optimized to achieve room temperature compensation and zero saturation magnetization. This property enables PMA garnet-based room temperature terahertz magnonics. The lattice parameters of GdIG (af=12.480Å) and SGGG (as=12.48Å) match exactly, so the in-plane strain value is zero and the effect of Keff is eliminated completely. Consequently, due to small value for Ms of GdIG, shape anisotropy (3.98 ×102 erg·cm-3) cannot compete with magnetocrystalline anisotropy (-4.1×103 erg·cm-3) since it is not negligible. Consequently, the Keff is negative for GdIG when grown on SGGG due to the influence of magnetocrystalline anisotropy energy density. One other candidate for a PMA REIG on SGGG substrate is SmIG. Since af >as, compressive strain (-3.99 ×10-3) is induced in the film such that Kindu<0 possesses a value of an order of magnitude (-1.45×105 erg·cm-3) comparable to the Kshape (1.23×105 erg·cm-3). With its relatively large magnetocrystalline anisotropy energy density (-1.74×104 erg·cm-3), SmIG has a PMA due to negative value for effective anisotropy energy density (-4.80×105 erg·cm-3). TbIG film on SGGG substrate is a PMA candidate with positive strain and this film was also recently experimentally demonstrated to have PMA . Since TbIG’s lattice constant is smaller than that of the substrate, the film becomes subject to tensile strain (+1.61 ×10-3). Since TbIG also has a positive λ111 (in contrast to that of SmIG), the film’s ME anisotropy term becomes large and negative and overcomes the shape anisotropy. In case of TbIG, magnetocrystalline anisotropy alone overcomes shape and renders the film PMA on SGGG. With the additional Kindu contribution (-8.14×104 erg·cm-3), significant stability of PMA can be achieved. Terbium Gallium Garnet (TGG) is a substrate with lattice parameter (as=12.355Å) such that it can induce tensile strain on TmIG, ErIG and YbIG and it induces compressive strain on the rest of the REIG (YIG, DyIG, HoIG, TbIG, GdIG, SmIG, EuIG). In none of the tensile-strained cases, PMA can be achieved since the Kindu>0 and has the same sign as the Kshape. Among the compressively strained cases, YIG, TbIG and EuIG are found to have weak ME anisotropy terms which cannot overcome shape. As a result, YIG, TbIG and EuIG on TGG substrate are expected to have in-plane easy axis. DyIG, HoIG, GdIG and SmIG films on TGG achieve large and 11
negative Keff due to their negative λ111 values. In addition, since the materials have compressive strain, large and negative Kindu can overcome Kshape in these materials. So these cases are similar to the conditions explained for GGG substrate, on which only DyIG, HoIG, GdIG, and SmIG films with PMA. Neodymium gallium garnet (NGG) is another substrate 45 used for growing garnet thin films by PLD method. NGG has large lattice constant compared with the rest of the bulk REIG and yield compressive strain in all investigated except for SmIG. For all cases other than SmIG, the sign of the magnetoelastic anisotropy term is determined by the respective λ111. YIG, TmIG, DyIG, HoIG, ErIG, YbIG have Kindu>0, which lead to easy axes along their film planes. For SmIG and EuIG on NGG, Kindu is not large enough to overcome large shape anistropy. For GdIG, the weak tensile strain on NGG actually causes in-plane easy axes because Kindu offsets the negative magnetocrystalline anisotropy. The only REIG that can achieve PMA on NGG is Terbium Iron Garnet (TbIG) due to its large negative Kindu (-2.44×105 erg·cm-3 ) which can offset Kshape (1.59×103 erg·cm-3) and K1 term (-8.20×103 erg·cm-3). Consequently, we predict that growing TbIG on NGG substrate may yield PMA (Keff= -2.51×105 erg·cm-3). Fig. 3 shows the substrates on which one may expect PMA rare earth iron garnet films (or negative Keff) due to strain only. Fig.s 3(a)-(d) compare the calculated effective energy densities as a function of strain type and sign for YIG, TmIG, YbIG, TbIG. For comparing the calculation results presented here with the experimentally reported values for the Keff of TmIG, we added the Keff directly from the experimental data in  to Fig. 3(b). As shown on Fig. 3(b), the experimental TmIG thin film shows positive Keff as the result of tensile in-plane strain and large negative magnetostriction constant. Fig. 4(a)-(f) Keff as a function of strain type and sign for GdIG, SmIG, EuIG, HoIG, DyIG, ErIG, respectively. Keff may get a positive or a negative value in both compressive and tensile strain cases due to varying signs of λ111 constants of REIG. In almost all cases that yield PMA on the given substrates, PMA iron garnets form under compressive lattice strain. The only exceptions in which tensile strain can yield PMA in garnet thin films is TbIG on SGGG and TbIG on NGG. In both of those cases, a small tensile strain enhances PMA but the magnetocrystalline anisotropy could already overcome shape and yield PMA without lattice strain. Therefore, experimental studies should target compressive lattice strain.
Fig. 3. Effect of substrate strain on the effective anisotropy energy densities of (a) YIG, (b) TmIG, the data inserted on the graph, with red square symbol, GGG (Exp.), is the experimental value of effective anisotropy energy of TmIG on GGG based on Ref. (c) YbIG, (d) TbIG. Note that the axes scales are different in each part.
Fig.4. (a) GdIG, (b) SmIG, (c) EuIG, (d) HoIG, (e) DyIG, (f) ErIG films on GGG, YAG, SGGG, TGG, and NGG substrates. Note that the axes scales are different in each part.
Based on Fig. 2-4, the calculations in this paper numerically match with the reported values in the experimental demonstrations in literature both in sign and order of magnitude. However, since there are inconsistent sign conventions for predicting the magnetic anisotropy state of the iron garnet samples in the literature so far, some of the previous studies draw different conclusions on the anisotropy despite the similar Keff. We tested the prediction accuracy of our model by going through each experimental demonstration of garnet thin film/substrate anisotropy and comparing their measured anisotropies with the predictions of our model. In Data in Brief document, we show the prediction accuracy and cases where experiments are different from our predictions. The model presented here could accurately predict the magnetic anisotropy state in almost all cases of garnet film/substrate combinations. The partial differences between our predictions and the experimental outcomes in a few cases arise from the deviation of experimentally measured film parameters from the tabulated properties used in our model (like Ms, λ111, strain, Young’s modulus, Poisson’s ratio). In almost all pairs among 20 predicted PMA cases, the model can accurately predict the anisotropy state if the material properties are accurately entered in the model. In case of TmIG, as shown in Fig. 3(b), our model predicts that there is a tensile strain-induced anisotropy resulting from the difference in film and substrate lattice parameters and the film’s negative magnetostriction constant. The experimental results of magnetic anisotropy in TmIG/GGG [7, 18, 46] are consistent with our model predictions. Previous studies identify PMA, if the film Keff is positive. A shortcoming of this approach is that such a definition would also identify YIG/GGG as PMA, although its in-plane easy axis behavior has been experimentally demonstrated in numerous studies [3, 32, 47]. Keff < 0 for PMA definition would be thermodynamically more appropriate and would also accurately explain almost all cases including YIG/GGG. Further explanation about TmIG exceptional case is included in the Data in Brief. 3.2. Sensitivity of Anisotropy to Variations in Saturation Magnetic Moment and Film Relaxation The films with predicted effective anisotropy energy and field may come out differently when fabricated. It is due to unintentional variability in fabrication process conditions, film stoichiometry (rare earth ion to iron ratio and oxygen deficiency) as well as process-induced nonequilibrium phases in the garnet films. These changes may partially or completely relax the films or increase strain further due to secondary crystalline phases. Practical minor changes in strain may dramatically alter both the sign and the magnitude of magnetoelastic anisotropy energy and may cause a film predicted as PMA to come out with in-plane easy axis. On the other hand, offstoichiometry may cause reduction in saturation magnetic moment. Reduction in saturation magnetic moment decreases shape anisotropy term quadratically (Kshape = 2πMs2), which implies that a 10% reduction in Ms leads to a 19% decrease in Kshape; and anisotropy field may increase (HA = 2Keff/Ms). Therefore, sample fabrication issues and the consequent changes in anisotropy terms may weaken or completely eliminate the PMA of a film/substrate pair and alter anisotropy field. While these effects may arise unintentionally, one can also use these effects deliberately for 15
engineering garnet films for devices. Therefore, the sensitivity of anisotropy properties of garnet thin films such as anisotropy field and effective anisotropy energy density needs to be evaluated with respect to changes in film strain and saturation magnetic moment. Fig.5 shows the sensitivity of the Keff to deviation of both strain and, Ms for five PMA film/substrate combinations: (a) HoIG/GGG, (b) YIG/YAG, (c) SmIG/SGGG, (d) HoIG/TGG, and (e) SmIG/NGG). The change of anisotropy energy from negative to positive indicates a transition from PMA to in-plane easy axis. In these plots, calculated anisotropy energies are presented for Ms and strains of fully lattice-matched films on the substrates scanned from 60% to 140% of tabulated bulk Ms and strains for tabulated lattice constants. The color scale indicates the anisotropy energy density in erg·cm-3. A derivation of anisotropy energy as a function of Ms and strain in Eq.s (8)-(10) shows that the negative λ111 values and negative strain states (compressive strain) for garnet films in Fig. 5(a)-(e) (HoIG, YIG, SmIG) enable these films to have PMAThe necessary condition for maintaining PMA is shown in Eq.11. (8)
Keff = Kindu + Kshape + K1 3
Keff = ― 2λ1111 ― vε|| +2πMs2 + K1 3
Keff = 2λ1111 ― v|ε||| + 2πMs2 + K1 Keff < 0 if
|ε||| + K1| > 2πMs2
(9) (10) (11)
Relaxing each fully strained and lattice-matched thin film towards unstrained state (ε → 0 or moving from left to right on each plot in Fig. 5) causes the Kindu to decrease in magnitude and gradually vanish. The total anisotropy energy decreases in intensity for decreasing strain and constant Ms. When Ms increases, shape anisotropy term also increases and overcomes Kindu. As a result, higher Ms for relaxed films (i.e. relatively thick and iron-rich garnets) may lose PMA. Therefore, one needs to optimize the film stoichiometry and deposition process conditions, especially growth temperature, oxygen partial pressure and film thickness, to ensure that the films are strained and stoichiometric. Since strains are less than 1% in Fig. 5(a), 5(c)-(e), these samples are predicted to be experimentally more reproducible. For YIG on YAG, as shown in Fig. 5(b), the strains are around 3%, which may be challenging to reproduce. The cases presented in Fig. 5(a)-(e) are the only cases among 50 film/substrate pairs where reasonable changes in Ms and strain may lead to complete loss of PMA. The rest of the cases have not been found as sensitive to strain and Ms variabilities and those predicted to be PMA are estimated to have stable anisotropy. Effective anisotropy energy plots similar to Fig. 5(a)-(e) are presented in the Data in Brief figures for all 50 film/substrate pairs. While PMA is a useful metric for garnet films, the effective anisotropy energy of the films should also not be too high (< a few 105 erg·cm-3) otherwise the saturation fields for these films would reach or exceed 0.5 Tesla (5000 Oe). Data in Brief figures present the calculated Keff and HA 16
values for all 50 film/substrate pairs for changing strain and Ms values. These figures indicate that one can span anisotropy fields of about 300 Oersteds up to 12.6 Tesla in PMA garnets. For practical integrated magnonic devices, the effective anisotropy energy should be large enough to have robust PMA although it should not be too high such that effective anisotropy fields (i.e. saturation fields) would still be small and feasible. Engineered strain and Ms through controlled oxygen stoichiometry may help keep anisotropy field low while retaining PMA. In addition, according to the recently published paper on magnetic anisotropy of HoIG , the lattice matching in case of the thick samples becomes challenging to sustain, and the strain relaxes inside the film. Thus, the decrease in the anisotropy field is one consequences of the lower strain state, which is an advantage for magnonics or spin-orbit torque devices. Below a critical thickness, HoIG grown on GGG has PMA. However, as the film reaches this critical thickness, the 40% or more strain relaxation is expected and the easy axis becomes in-plane. So thinner films are preferred to be grown in integrated device applications.
Fig. 5. Effect of partial film relaxation and saturation magnetic moment variability on the effective anisotropy energy density of the films. Variation of effective magnetic anisotropy energy densities for (a) HoIG on GGG, (b) YIG on YAG, (c) SmIG on SGGG, (d) HoIG on TGG and (e) SmIG on NGG are presented when strain relaxation and magnetic saturation moments change independently. Film strain may vary from a completely lattice-matched state to the substrate to a relaxed state or a highly strained state due to microparticle nucleation. Strain variability alters magnetoelastic anisotropy and cause a PMA film become in-plane easy axis. On the other hand, magnetic saturation moments may deviate from the 18
tabulated values because of process-induced off-stoichiometry in the films (i.e. rare earth ion to iron ratio or iron deficiency or excess, oxygen deficiency). Relaxing the films reduces the magnetoelastic anisotropy term and diminishes PMA. Increasing Ms strengthens shape anisotropy and eliminates PMA for low enough strains for all five cases presented.
Minimizing Gilbert damping coefficient in garnet thin films is also an important goal for spintronic device applications. First principles predictions of physical origins of Gilbert damping  indicate that magnetic materials with lower Ms tend to have lower damping. Based on this prediction, DyIG, HoIG and GdIG films are predicted to have lower Gilbert damping with respect to the others. Since the compensation temperatures of these films could be engineered near room temperature, one may optimize their damping for wide bandwidths all the way up to terahertz (THz)  spin waves or magnons. The first principles predictions also indicate that higher magnetic susceptibility (χm) in the films helps reduce damping (i.e. lower saturation field). Therefore, the PMA garnet films with lower anisotropy fields are estimated to have lower Gilbert damping parameters compared to PMA garnets with higher anisotropy fields. 4. Conclusion Shape, magnetoelastic and magnetocrystalline anisotropy energy terms have been calculated for ten different garnet thin films epitaxially grown on five different garnet substrates. Negative Keff (effective magnetic anisotropy energy) corresponds to perpendicular magnetic anisotropy in the convention used here. 20 different garnet film/substrate pairs have been predicted to exhibit PMA and their properties are listed on Table 2. By choosing a substrate with a lattice parameter smaller than that of the film, one can induce compressive strain in the films to the extent that one can always overcome shape anisotropy and achieve PMA for large and negative λ111. Among the PMA films predicted, SmIG possesses a high anisotropy energy density and this film is estimated to be a robust PMA when grown on all five different substrates. To obtain PMA, magnetoelastic anisotropy must be large enough to overcome shape anisotropy. Both compressive and tensile-strained films can become PMA as long as shape anisotropy can be overcome with large magnetoelastic strain. Here, in almost all cases, iron garnets come out with PMA under compressive film strain, except TbIG on SGGG and TbIG on NGG. These two cases have tensile strain and relatively large magnetocrystalline anisotropy, which could already overcome shape anisotropy without strain. We suggest experiments to achieve compressive lattice strain in most garnets for PMA. Among the 20 PMA cases, HoIG/GGG, YIG/YAG, SmIG/SGGG, HoIG/TGG and SmIG/NGG cases have been found to be sensitive to fabrication process or stoiochiometry-induced variations in Ms and strain. Among the cases predicted to possess PMA, anisotropy fields ranging from 310 Oe (0.31 T) to 12.6 T have been calculated. Such a wide anisotropy field range could be spanned and engineered through strain state, stoichiometry as well as substrate choice. For integrated magnonic devices and circuits, garnets with low Ms and lower anisotropy fields (HA < 0.5 T) 19
would require less energy for switching and would be more appropriate due to their lower estimated Gilbert damping. Our model has highlighted the sensitivity of magnetic anisotropy to the films’ magnetic and structural properties. Due to this sensitivity, we believe more precise and explicit reporting of experimental characterization results of film properties could help understand anisotropy much better. Acknowledgments M.C.O. acknowledges BAGEP 2017 Award and TUBITAK Grant No. 117F416. Appendix A. Supplementary Data Supplementary data associated with this article can be found online as Data in brief. Competing interests There is no financial and non-financial competing interest among the authors. Author contributions M.C.O. designed the study. S.M.Z. performed the calculations and evaluated and analyzed the results with M.C.O. Both authors discussed the results and wrote the manuscript together.
References                    
Avci, C.O., et al., Current-induced switching in a magnetic insulator. Nature Materials, 2017. 16(3): p. 309. Chumak, A., et al., Magnon spintronics. Nature Physics, 2015. 11(6): p. 453. Onbasli, M., et al., Pulsed laser deposition of epitaxial yttrium iron garnet films with low Gilbert damping and bulk-like magnetization. APL Materials, 2014. 2(10): p. 106102. Serga, A., A. Chumak, and B. Hillebrands, YIG magnonics. Journal of Physics D: Applied Physics, 2010. 43(26): p. 264002. Garello, K., et al., Ultrafast magnetization switching by spin-orbit torques. Applied Physics Letters, 2014. 105(21): p. 212402. Kalashnikova, A., et al., Magneto-optical study of holmium iron garnet Ho3Fe5O12. Low Temperature Physics, 2012. 38(9): p. 863-869. Kubota, M., et al., Stress-induced perpendicular magnetization in epitaxial iron garnet thin films. Applied Physics Express, 2012. 5(10): p. 103002. Maier-Flaig, H., et al., Perpendicular magnetic anisotropy in insulating ferrimagnetic gadolinium iron garnet thin films. arXiv preprint arXiv:1706.08488, 2017. Tang, C., et al., Above 400-K robust perpendicular ferromagnetic phase in a topological insulator. Science Advances, 2017. 3(6): p. e1700307. Wang, H., et al., Strain-tunable magnetocrystalline anisotropy in epitaxial Y3Fe5O12 thin films. Physical Review B, 2014. 89(13): p. 134404. Yamahara, H., et al., Epitaxial strain-induced magnetic anisotropy in Sm3Fe5O12 thin films grown by pulsed laser deposition. Journal of Magnetism and Magnetic Materials, 2011. 323(23): p. 3143-3146. Adam, J.D., et al., Ferrite devices and materials. IEEE Transactions on Microwave Theory and Techniques, 2002. 50(3): p. 721-737. Calhoun, B., J. Overmeyer, and W. Smith, Ferrimagnetic resonance in gadolinium iron garnet. Physical Review, 1957. 107(4): p. 993. Dionne, G.F., Molecular field and exchange constants of Gd3+‐substituted ferrimagnetic garnets. Journal of Applied Physics, 1971. 42(5): p. 2142-2143. Fu, J., et al., Epitaxial growth of Y3Fe5O12 thin films with perpendicular magnetic anisotropy. Applied Physics Letters, 2017. 110(20): p. 202403. Popova, E., et al., Perpendicular magnetic anisotropy in ultrathin yttrium iron garnet films prepared by pulsed laser deposition technique. Journal of Vacuum Science & Technology A: Vacuum, Surfaces, and Films, 2001. 19(5): p. 2567-2570. Kubota, M., et al., Systematic control of stress-induced anisotropy in pseudomorphic iron garnet thin films. Journal of Magnetism and Magnetic Materials, 2013. 339: p. 63-70. Quindeau, A., et al., Tm3Fe5O12/Pt heterostructures with perpendicular magnetic anisotropy for spintronic applications. Advanced Electronic Materials, 2017. 3(1): p. 1600376. Soumah, L., et al., Ultra-low damping insulating magnetic thin films get perpendicular. Nature Communications, 2018, 9, 3355. Monzon, F., D. Patterson, and M. Roukes, Characterization of individual nanomagnets by the local Hall effect. Journal of Magnetism and Magnetic Materials, 1999. 195(1): p. 1925.
                     
Park, J.-H., et al., Magnetic softening of switching field of magnetic garnet films by controlling groove depth. Journal of Applied Physics, 2003. 93(10): p. 8522-8524. Zhu, N., et al., Patterned growth of crystalline Y3Fe5O12 nanostructures with engineered magnetic shape anisotropy. Applied Physics Letters, 2017. 110(25): p. 252401. Bobeck, A., et al., Uniaxial magnetic garnets for domain wall "BUBBLE'' devices. Applied Physics Letters, 1970. 17(3): p. 131-134. Li, X., et al., Controllably manipulating three-dimensional hybrid nanostructures for bulk nanocomposites with large energy products. Nano Letters, 2017. 17(5): p. 2985-2993. Chen, J., et al., Spin wave propagation in perpendicularly magnetized nm-thick yttrium iron garnet films. Journal of Magnetism and Magnetic Materials, 2018. 450: p. 3-6. Duan, M., et al., Laser deposited bismuth doped iron garnet films with perpendicular anisotropy. IEEE Transactions on Magnetics, 1995. 31(6): p. 3245-3246. Suchomski, C., et al., Large-pore mesoporous Ho3Fe5O12 thin films with a strong roomtemperature perpendicular magnetic anisotropy by sol–gel processing. Chemistry of Materials, 2014. 26(7): p. 2337-2343. DA, W., et al., Preparation and characterization of Bi substituted gadolinium iron garnet BixGd3-xFe5O12 films with x= 1 to 2.5 by enhanced metal organic decomposition method. Journal of the Magnetics Society of Japan, 2016. 40(4): p. 107-114. Park, I.J., K.U. Kang, and C.S. Kim, Temperature-dependent magnetic properties of bismuth substituted terbium–iron garnets. IEEE Transactions on Magnetics, 2006. 42(10): p. 2882-2884. Guo, H., et al., Strain doping: Reversible single-axis control of a complex oxide lattice via helium implantation. Physical Review Letters, 2015. 114(25): p. 256801. Guillot, M., et al., High magnetic field properties of mixed terbium-yttrium ferrite garnets. Zeitschrift für Physik B Condensed Matter, 1989. 74(3): p. 335-339. Lang, M., et al., Proximity induced high-temperature magnetic order in topological insulator-ferrimagnetic insulator heterostructure. Nano Letters, 2014. 14(6): p. 34593465. Iida, S., Magnetostriction constants of rare earth iron garnets. Journal of the Physical Society of Japan, 1967. 22(5): p. 1201-1209. Von Aulock, W.H., Handbook of microwave ferrite materials. 1965. Paoletti, A., Physics of magnetic garnets: Proceedings of the international school of physics' Enrico Fermi', Course LXX, Varenna on Lake Como, Villa Monastero, 27th June-9th July 1977. 1978: Elsevier Science & Technology. Tang, C., Materials development and spin transport study of magnetic insulator based heterostructures. 2017: Ph.D. Dessertation, University of California, Riverside. Sander, D., The correlation between mechanical stress and magnetic anisotropy in ultrathin films. Reports on Progress in Physics, 1999. 62(5): p. 809. Dionne, G.F., Magnetic oxides. Vol. 14. 2009: Springer, NewYork. Geller, S., et al., Magnetic study of the lighter rare-earth ions in the iron garnets. Physical Review, 1963. 131(3): p. 1080. Dodrill, B., Lindemuth, J. & Krause, J. Magnetic anisotropy: Measurements with a vector vibrating sample magnetometer, www.lakeshore.com/Documents. Huber, D., B. Magnetoelastic properties of the iron garnets, in Part A. 1970, Springer, Berlin, Heidelberg. p. 346-348. Nakamoto, R., et al., Properties of rare-earth iron garnets from first principles. Physical Review B, 2017. 95(2): p. 024434. 22
       
Yoshimoto, T., et al., Static and dynamic magnetic properties of single‐crystalline yttrium iron garnet films epitaxially grown on three garnet substrates. Advanced Electronic Materials, 2018. 4(7): p. 1800106. Li, G., et al., Tunable perpendicular magnetic anisotropy in epitaxial Y3Fe5O12 films. APL Materials, 2019. 7(4): p. 041104. Rosenberg, E.R., et al., Magnetism and spin transport in rare-earth-rich epitaxial terbium and europium iron garnet films. Physical Review Materials, 2018. 2(9): p. 094405. Wu, C., et al., High-quality thulium iron garnet films with tunable perpendicular magnetic anisotropy by off-axis sputtering–correlation between magnetic properties and film strain. Scientific Reports, 2018. 8(1): p. 11087. Goto, T., M.C. Onbaşlı, and C.A. Ross, Magneto-optical properties of cerium substituted yttrium iron garnet films with reduced thermal budget for monolithic photonic integrated circuits. Optics Express, 2012. 20(27): p. 28507-28517. Zanjani, S.M. and M.C. Onbasli, Thin film rare earth iron garnets with perpendicular magnetic anisotropy for spintronic applications. AIP Advances, 2019. 9(3): p. 035024. Hickey, M.C. and J.S. Moodera, Origin of intrinsic Gilbert damping. Physical Review Letters, 2009. 102(13): p. 137601. Geprägs, S., et al., Origin of the spin Seebeck effect in compensated ferrimagnets. Nature Communications, 2016. 7: p. 10452.
The anisotropy energies of 10 different types of iron garnet compounds epitaxially grown and latticematched as thin films (X3Fe5O12, X = Y, Tm, Dy, Ho, Er, Yb, Tb, Gd, Sm, Eu) on commercially available (111)-oriented garnet substrates (Gd3Ga5O12 or GGG, Y3Al5O12 or YAG, Gd3Sc2Ga3O12 or SGGG, Tb3Ga5O12 or TGG, Nd3Ga5O12 or NGG).
We calculated the shape, magnetocrystalline and magnetoelastic anisotropy energy densities for these lattice-matched 50 cases.
We found that in 20 cases out of 50, magnetoelastic anisotropy overcomes shape and render these film/substrate pairs as candidates for room temperature PMA.
Only 7 of these 20 PMA cases have been experimentally directly verified.
Our study highlights that one can achieve room temperature PMA in a variety of rare earth iron garnets with different saturation, coercivity, Gilbert damping and compensation temperatures. Most of these PMA cases are robust against partial film relaxation and variations in saturation magnetic moment.